The topic in this chapter concerns organic nanocrystals. Numerous scientific researches of nanocrystals are focusing on inorganic compounds such as a metal and a semiconductor. The research related to organic nanocrystals is relatively new compared to that of inorganic nanocrystals. Nearly two decades ago, our research team had developed a novel preparation method of organic nanocrystals, what we call the reprecipitation method. Since then, we have been leading the research area of organic nanocrystals. The reprecipitation method has bottom-up type with a wet process procedure to prepare organic nanocrystals, and organic nanocrystals are obtained as their water dispersion. Numerous numbers of organic compounds are allowed to be a candidate for a targeting of organic nanocrystals by means of using the reprecipitation method. Functional organic nanocrystals have been attracted in a scientific and technological area of materials. In this chapter, first we mention the research back ground of organic nanocrystals, and then introduce the preparation method of organic nanocrystals, i.e. the reprecipitation method, and their improved ones. Then, several kinds of functional organic nanocrystals relating to optoelectrical materials, nanomedicine, and biophotonics are mentioned. Recent topics of organic nanocrystals achieved by several groups are briefly introduced. In this chapter, the topics are proceeding as follows:
Back ground of the research of organic nanocrystals
Preparation method of organic nanocrystals
Several functional organic nanocrystals
Recent topics of organic nanocrystals achieved by several groups
2. Back ground of the research of organic nanocrystals
Fabrication of nanocrystals and their nanostructure has been investigated extensively for metals (Ung et al., 1997) and semiconductors (Murray et al., 1993), and many characteristic properties have already been shown. For example, a novel and unique optical property called the quantum size effect (Nakamura, 1992) was found for such inorganic nanocrystals in a size of a few nanometres (e.g. nonlinear optics, semiconductor lasing, and quantum dot applications).
For organic nanocrystals, however, nanocrystals fabrication has so far rarely been investigated, owing to their thermal instability, except for the thermally stable phthalocyanine and a kind of low molecular weight aromatic compounds which were nanocrystallized by an evaporation method in an inert gas (Granqvist et al., 1976) or by a crystal growth technique in a porous polymer (Matsui et al., 1995). Recently, we have proposed a simple and convenient method for the fabrication of organic nanocrystals, what we call the reprecipitation method (Kasai et al., 1992). In brief, the hydrophobic solution in which hydrophobic compounds dissolved is injected into water, which results in a reprecipitation owing to its insolubility in water to give nanocrystal dispersion. By this method, many kinds of organic compounds such as polydiacetylene (Katagi et al., 1996), phthalocyanine (Yanagawa et al., 1997), perylene (Kasai et al., 1996) and so on can be nanocrystallized successfully. Interestingly, size-dependent optical properties are observed for these organic nanocrystals even in the 100 nm size range, an order of magnitude larger than the scale where the inorganic nanocrystals usually show size-dependent optical properties. These aqueous organic nanocrystals dispersions may have great potential for use in fundamental and applied optics, e.g. as nonlinear optical (NLO) materials having large
Until now, not only the investigation of fundamental optelectrical properties of organic nanocrystals, but also their interesting physiochemical properties and their peculiar advantages compared to inorganic nanocrystals have been extended to nanomedicine and biophotonics. First we introduce the fabrication technique of organic nanocrystals; the reprecipitation method.
3. Preparation method of organic nanocrystals
3.1. The reprecipitation method
The reprecipitation method, which is a solvent displacement method, was first reported by our research groups (Fig. 1a) (Kasai et al., 1992). It provides a very simple and versatile way to prepare organic nanocrystals dispersions. The method involves a rapid mixing of a smallamount of concentrated stock solution of the target compound dissolved in a good solvent with excess of a poor solvent. The great disparity between the solubilities of the target compound in the good and poor solvents, and the good compatibility of the two solvents are essential for this method. The rapid mixing of the stock solution and the poor solvent changes the micro-environment of the target compound molecules. The molecules are exposed to the poor solvent surroundings in a very short time, inducing the nucleation and growth of the molecules to nanocrystals. The size and morphology of nanocrystals can be controlled (Fig. 1 b and 1c) by tuning a concentration, temperature, stirring speed, and adding surfactant. Then the precipitation creates nanocrystals dispersed in water. Many kinds of organic compound such as π-conjugate compounds, NLO dyes (Kaneko et al, 2005), fluorescent dyes (Fig. 1d), fullerene (Tan et al., 2008), and several polymers (Ishizaka et al., 2006; Zhao et al., 2009) are candidate for nanocrystals (nanoparticles for polymer). However some kinds of rigid compounds such as phthalocyanine having π-π stack structure are quite hard to be solved in usual organic solvent, thus for the nanocrystal preparation of these attractive functional compound, an advanced preparation technique is required. A supercritical fluid is a candidate for dissolving this problem.
3.2. Supercritical fluid crystallization method
The properties of phthalocyanine are very interesting in both optics and electronics in the fields of nonlinear optics, organic photoconductors, and pigments. Phthalocyanine is known
to have large
On the other hand, supercritical fluid (SCF) has been expected to have a high solubility against insoluble organic compounds, since it shows high solubility under high temperatures and high pressure. Thus, we expected the SCF approach to be an alternative method for making phthalocyanine nanocrystals, instead of the acid pasting method. On the basis of this idea, the use of SCF was examined for the purpose of improving the reprecipitation method. The new method is called supercritical fluid crystallization (SCFC) method (Fig. 2) (Komai et al., 1998). The preparation of phthalocyanine nanocrystals using the SCFC method was used in order to demonstrate this usefulness. The size and modification control of titanyl phthalocyanine crystal have been attempted using the reprecipitation method from SCFC. The fabrication
3.3. Microwave-irradiation reprecipitation method
Recently, as a novel fabrication technique of functional materials, a microwave irradiation process is much noted in the field of organic and inorganic synthesis and nanoparticles. For example, high critical temperature superconductors, mono-dispersed nickel, gold, silver nanoparticles, and organic-metal complexes were successfully prepared by using this technique.
We focused on the unique aspect of microwave at 2.45 GHz. One of the aspects of microwave (2.45 GHz) is that the microwave is well absorbed by water molecule, resulting in effective homogeneous and rapid heating of water is realized. Since nanocrystals are prepared in water environment by the reprecipitation method, we have attempted to apply the microwave-irradiation process to the reprecipitation method for the purpose of fabricating well-defined organic nanocrystals (Fig. 3). Upon microwave-heating was applied
to the reprecipitation method, homogeneous and rapid heating increased the homogeneous crystal growth and then the crystallization was completed without particle aggregation. This homogeneous heating resulted in making fine narrow-sized homogeneous nanocrystals dispersed in water (Baba et al., 2000). If the conventional conductive heating such as hot plate heating was used, this gradient heating induced large-sized and random-size distributed crystal growth in aqueous dispersion system.
We demonstrated that the narrow size distributed nanocrystals of TPB, perylene (Fig. 4) (Baba et al., 2000), and DCHD were successfully fabricated within a short time by applying microwave heating just after our conventional reprecipitation procedure. Furthermore, there was finding that the size and morphology of DCHD nanocrystals and nanofiber were controlled well under using the open- and closed-type vessel (Fig. 5) (Baba et al., 2007a).
The next stage of our interest was how to mass produce these attractive organic nanocrystals for the sake of industrial approach.
3.4. Mass production of organic nanocrystals
The reprecipitation method is an easy and convenient technique to fabricate organic nanocrystals in general. However, only limited amount of nanocrystals dispersion (about several-tens ml) was prepared at once, i.e. the laboratory scale. To overcome this problem, we introduced a pump as an injection apparatus of the reprecipitation method for mass-production of pigment nanocrystals with controlled size and morphology (Ujiiye-Ishii et al., 2006).
For mass-production, most efficient conditions of the reprecipitation method have injecting highly concentrated solution with high injection rate. The former condition was achieved by using 1-methyl-2-pyrrolidone (NMP) and the latter was realized by using a high flow-rate pump. Using the injection pump-assisted reprecipitation method, the amount of obtained quinacridone nanocrystals in dispersion was 700 mg per minute at maximum, and then 3.5 g of the nanocrystals were obtained in one experiment. This value was about 17,500 times
larger than that obtained by the conventional reprecipitation method with manual injection. The size of quinacridone nanocrystals fabricated was 25–80 nm, which was confirmed by observation using a scanning electron microscope. From the powder X-ray diffraction data, only α-type nanocrystals were obtained. This mass production procedure of pigment nanocrystals is useful for an application of a color filter.
4. Several functional organic nanocrystals
4.1. Color filter using organic pigment nanocrystals
Organic pigments have been widely used in printing and coating industries as the coloring agents of synthetic fibers and plastics. Recent years, some organic pigments have an attention as organic photoconductors such as organic EL materials and electrophotographic photoreceptors. In addition, organic pigments are used for ink-jet inks to produce photographic-quality pictures and for color filters that are essential materials for the full-colorization of digital cameras and liquid crystal displays (LCDs). To increase the performance of the color filter, it is absolutely essential to cancel out the light scattering by reducing the particle size of organic pigments. Yet dyes can be an attractive alternative to overcome this limitation due to the reduced light scattering because they are dissolved in the media and exist in molecule form, however, in order for the dyes to be applied successfully to LCDs manufacturing process, their low thermal stability needs to be improved. Therefore, as the way to reduce the particle size, the breakdown method using beads and/or inorganic salts are commonly used. However, an energy efficiency, inclusion of contaminants such as bead materials (e.g., inorganic salts and zirconia), and a difficulty to reduce the particle size less than 50 nm are causing industrial problems. Therefore, the solution of these problems has been strongly desired. To overcome these problems, mass production procedure of organic pigment nanocrystals by the newly developed reprecipitation method was investigated, and the possibility of their application to color filter for LCDs was evaluated.
To evaluate the prepared organic pigment nanocrystals as a functional material for color filters, it is necessary to significantly increase their preparation amount. For this realization, a highly concentrated pigment solution and an improvement in the injection rate of the solution were necessary. Based on the literature (Ujiiye-Ishii et al., 2006), the system using a pulsation-free pump was built. In this newly developed reprecipitation method, it increased the preparation amount of nanocrystals by 104–106 times (Miyashita et al., 2008).
The organic pigment nanocrystals prepared by the reprecipitation method were finer in mono-dispersed property, compared to the conventional products. The average size of pigment nanocrystals prepared by the reprecipitation method was 25 nm and that of the pigments prepared by the breakdown improved milling method was 39 nm, and the former was in finer size dispersion (i.e., mono-dispersion). The relationship between the particle formation mechanism and particle size in the reprecipitation method is also under study. To clarify the reduction of the light scattering that is affected by the reduced size of pigment particles, the light scattering intensity was measured using a goniometer. In LCDs, if the light scattering occurs by pigment particles, the reduction of the display contrast and/or the luminance ratios occurs. Thus this becomes a serious problem when the display is in ON/OFF in LCDs.
It is apparent that the use of pigment nanocrystals prepared by the reprecipitation method can significantly increase the contrast ratio of LCDs, which is one of the most important performances. As a result, a new production process of organic pigment nanocrystals reduced the light scattering by fine size and well dispersed organic pigment nanocrystals prepared by the reprecipitation method.
It was found that organic pigment nanocrystals with the particle size about 25 nm were successfully achieved by the reprecipitation method. Because the fine size-controlled organic pigment nanocrystals lead to very little light scattering, they are considered to be useful for improving the performance of color filters that are an essential component of LCD.
4.2. Organic nanocrystals for organic field effect transistor
The functionality of organic pigment is attracted in electro devices such as organic electro luminescence devices and organic field effect transistor (OFET). Especially, the research of OFET is hot topic toward a future of optical device. Several kinds of electron-hole transfer organic compounds are well investigated. For OFET, carrier mobility is important factor for high quality devices. A π-conjugate polymer, polydiacetylene (PDA), is one of the promising compounds having high carrier mobility. PDA is a unique material, which combine the properties of an essentially one-dimensional, fully conjugated polymer with the ability of single crystalline monomers to polymerize without disruption of the crystallinity (Takahashi, et al., 2002). PDA has the optical properties of large non-linear optical susceptibility and ultra-fast response time as well as a PDA been predicted to present very high charge carrier mobility, up to 103–105 cm2/V s. However the real mobility of PDA crystals measured using time-of-flight technique was found to be 1–10 cm2/V s, and that is comparable to those measured on polyacene molecular crystals such as anthracene or naphthalene. The use of PDA films as an active layer of OFET is very promising task, however the pure electrical conductivity of these films have restricted their application. Thus to improve the conductivity is attracted work. Several attempts to improve the electrical conductivity have been reported; chemical doping into the stage of monomer crystals and in the course of solid-state polymerization, chemical doping into soluble polydiacetylenes, chemical doping into a Langmuir–Blodgett film of PDA, ion implantation to PDA bulk crystals, and using a scanning tunneling microscopy probe tip to fabricate linear PDA nanowires. Recently, the maximum conductivity for chemically doped PDA crystals has been reported to be as high as 10 2 S/cm. As a widely held opinion, one of the big issues in increasing the conductivity of PDA is that its rigid crystalline lattice prevents the dopant from penetrating into PDA bulk crystals. This was especially the case in 1,6-di-
To overcome the difficulty of chemical doping to PDA, we tried chemically doping into the nanocrystals of PDA, because PDA nanocrystals are known to have a softened crystal lattice (Baba, et al., 2006) and a large surface area, compared with bulk crystals, and demonstrated almost the highest conductivity of chemically doped PDA ever reported (Baba, et al., 2008). Figure 6 shows that the single layered poly-DCHD nanocrystals on slide glass and their specimen for measuring their conductivity. The success in chemical doping was achieved because poly-DCHD nanocrystals have a large surface area and softened crystal lattices, which allows chemical dopant species to diffuse easily into poly-DCHD nanocrystals in good contrast to the case of bulk crystals. Actually, nanostructure showed unique conformation change during solid state polymerization. Nanostructure have showed crack-less action during polymerization. This also showed that the nanocrystal has softened crystal lattice and has flexible stricture (this is mentioned in the next section). Thus, the PDA nanocrystals can accept the dopant. Aiming at the fully doped single crystalline nanocrystals of PDA, the effects of crystal size, morphology, and several kinds of chemical dopant species, which would increase the conductivity of PDA, are now under investigation.
As future approach, achieving the one dimensional array of the PDA nanofibers layered on the surface of devices is promising approach for high conductivity. We previously reported the one dimensional array of nanofibers. Furthermore, interesting finding concerning morphology changes during solid-state polymerization of PDA nanofibers were reported by our group, which related to topochemical study. This was because the softened crystal lattice of nanocrystals.
4.3. Solid state polymerization of polydiacetylene: topochemical polymerization
The research of the topochemical polymerization has been reported extensively since the 1960s, and PDA is the most attracted one. PDA also has been attracted because this π-conjugated polymer system has received much attention as conductive and non-linear optical materials. However, the accumulation of strain in bulk crystal during the solid-state
polymerization results in crushing crystal structure, and the rate of polymeric conversion does not occur with high efficiency. We found that the polymerization of nanocrystals achieved high quality polymeric crystal because the strain accumulated in nanocrystals was easily released (Baba, et al, 2006). Nanofibers prepared by the reprecipitation method had an average length of 10 μm and width of 50 nm. We found interesting behavior of morphological change of nanofibers during the stage of the solid-state polymerization. DCHD monomer nanofibers, which were fabricated by the reprecipitation method, were worm-like before solid-state polymerization. Interestingly, worm-like nanofibers converted into straight-like ones through the solid-state polymerization. This phenomenon indicated that the lattice in nanofibers was generally soft, compared with that of bulk crystals. The crystalline nanofibers are useful for the estimation of a nonlinear optical property and a conductivity of a single polymer chain.
4.4. Linear and nonlinear optical property of organic nanocrystals
PDA crystals have attractive nonlinear optical properties. Our interest is the nonlinearity occurred in nanocrystals. The fabrication of polydiacetylene nanocrystals with varied size was achieved using the reprecipitation method. The size effect on the absorption spectra, which was a characteristic to organic nanocrystals, has been experimentally verified. An important point is that size-dependent blue-shift appears at a size an order of magnitude larger than that of semiconductors and metals. That is due to the lattice vibration must become highly frequent with increasing temperature and also with decreasing crystal size. Actually, these thermal effects and sizes were clearly related to phonons in the nanocrystals lattice. The obtained
Photonic crystals have been a subject of considerable interest for more than a decade. A great deal of effort has been put into preparing highly ordered photonic crystals for the visible spectral range. Initial studies were directed toward the linear optical properties of these crystals, but more recent studies have focused on nonlinear processes in photonic crystals, and dramatic enhancements of these properties have been reported (Markowicz, et al., 2004).
Our interest is to study the optical properties of highly ordered 3-D arrays of polydiacetylene nanocrystals, since 3-D arrays formed by mono-dispersed particles in the range of 10 nm to 1 μm, referred to as colloidal crystals, show some special optical properties and potential applications, particularly in photonic devices. However, polydiacetylene nanoparticles are usually polyhedral and multi-dispersed. Their morphology prevents them from forming large-scale densely packed 3-D structures because the particles that form colloidal crystals are required to have a size variation of less than 5%. Polystyrene is one of the important materials in the fabrication of colloidal crystals, since uniform spherical polystyrene particles were easily synthesized by soap-free emulsion polymerization. When polydiacetylene nanocrystals are enclosed within uniform spherical polystyrene particles, the resulting composite particles are used to construct 3-D arrays of nonlinear materials. We reported the fabrication and characterization of spherical mono-dispersed composite particles consisting of 1,6-di(
Recently, an interest of photonic crystals has also been directed toward studying the effect of disorder in photonic crystals. Prasad’s group reported on a type of disorder in photonic crystals in which only a random variation of refractive index is introduced, without creating any structural or positional disorder, which was referred to be such disordered photonic crystals as photonic crystal alloys (Tiryaki, et al., 2004). The vertical deposition colloidal crystal method to produce three-dimensional photonic crystal alloys of polystyrene and poly(methyl methacrylate), 300 nm spheres in varying compositions were used. This photonic crystal alloys provided a convenient medium to compositionally tune the bandgap and the wavelength of a phase-matched nonlinear optical response. Prasad’s group is saying that the use of photonically active components (such as dye-doped spheres) allows one to conveniently create microcavities and study cavity electrodynamics.
4.5. Nanomedicine: Drug delivery system using drug nanocrystals
Numerous commonly used pharmaceutical drugs are hydrophobic in nature. Thus, special formulations are required to make their aqueous dispersion for these drugs delivery. Usually, surfactants or other nanoparticle-based delivery vehicles are used. Once systemic administration of these drugs, if the drug target cancer organ, such drug-doped carriers are preferentially taken up by tumour tissues based on the “enhanced permeability and retention effect”. The carriers include liposomes, polymeric micelles, oil dispersions (micelles), ceramic, hydrophilic drug−polymer complexes and polymeric nanoparticles. However many surfactants themselves tend to increase the systemic toxicity of the drug formulation. Therefore, there is increasing interest in the development of novel drug formulation and delivery methods without any external agents such as surfactants or other carrier vehicles. One method proposed for dispersion of hydrophobic compound in water, the reprecipitation method was used as demonstration.
Prasad’s group have prepared the nanocrystal formulation of a hydrophobic drug for photodynamic therapy (PDT) and compared its efficacy with the conventional surfactant-based formulation (Baba, et al., 2007b). PDT is a promising new modality for the treatment of a variety of cancers and some dermatological and ophthalmic diseases. The main advantage of PDT is the capability to localize the treatment, by using selective light exposure to the tumor site. Typical PDT treatment involves systemic administration of a photosensitizer drug, then localized light exposure at the tumor site using near-infrared light. After being excited with light, these photosensitizer molecules can transfer their excited-state energy to molecular oxygen in the surroundings, forming reactive oxygen species such as singlet oxygen. The locally generated reactive oxygen species destruct various cellular compartments, resulting in irreversible damage to tumor cells. The major disadvantage for successful clinical PDT is the poor water solubility of photosensitizing drugs. Thus, making their stable formulation for systemic administration is highly challenging. To overcome this difficulty, a stable dispersion of these drugs into aqueous systems is achieved using delivery vehicles. However, allergic reactions and their sustained
There was interesting finding that though the fluorescence and photodynamic activity of the drug nanocrystals were initially quenched in aqueous media. However, both recovered under
These results have not only mentioned the potential of using pure drug nanocrystals for PDT, but also this approach eliminates the need of any external agents such as surfactants or other carrier vehicles for drug delivery. Further studies are expected to increase the efficacy of nanocrystals by controlling their size that may affect long-term
4.6. Bioimaging using fluorescent dye nanocrystals
Fluorescence microscopy is one of the most versatile imaging techniques in biomedical research. That allows the non-invasive imaging of cells and tissues with molecular specificity. Such imaging requires a fluorescent dye to enter cells and tissues prior to visualization. Currently used dyes include members of the coumarin, rhodamine, fluorescein, and carbocyanine families. One of them, 3,3’-Dioctadecyloxacarbocyanine perchlorate [DiO; DiOC18(3)] is the long-chain dialkylcarbocyanine dye, and most commonly used for the visualization of anterograde and retrograde neuronal tracers in living cells. This lipophilic carbocyanine is also employed in many other applications, including cytotoxicity assays, the labeling of lipoproteins, and the tracking of cell migration and lipid diffusion in membranes through fluorescence recovery after photobleaching. The hydrophobic nature of these dyes means that, in many cases, organic solvents [e.g., dimethylformamide, dimethylsulfoxide (DMSO)] and surfactants are required for successful cell imaging. However, unfortunately, organic solvents and surfactants themselves tend to increase cytotoxicity
In addition to DiO dyes, many other fluorescent dyes are hydrophobic in nature—including perylene, a widely studied hydrophobic material that functions with a high quantum yield in organic electroluminescence devices. Although it is potentially useful for bioimaging, the preparation of aqueous dispersions of perylene dyes requires special formulation techniques, similar to those for DiO. The reprecipitation method was used to solvent-free and non-invasive bioimaging. We reported an organic solvent-free bioimaging method employing fluorescent dye nanocrystals prepared using the reprecipitation method and their application to
These nanocrystal formulations allowed efficient fluorescence confocal imaging of living cells
4.7. Thermoresponsive behaviour of fluorescent organic nanocrystals
After the first introduction of a temperature-responsive polymer, poly(
temperature of the cloud point, the polymer shows phase separation. The hydrophobic groups in the polymer form insoluble aggregates, turning the solution cloudy (Chen & Hoffman, 1995). Using this characteristic of PNIPAM, fluorescent dyes covalently linked to PNIPAM showed on-off fluorescent switching properties above and below the critical temperature. On the other hand, we demonstrated the thermoresponsive behaviour of fluorescent organic nanocrystals using PNIPAM in an aqueous system for the first time (Baba, et al., 2011). For the preparation of thermoresponsive fluorescent organic nanocrystals, fluorescent dyes of perylene, quinacridone, and zinc phthalocyanine were used. As a result, an on-off switching of fluorescence intensity was observed below and above around cloud point (~35 C). This thermoresponsive behaviour of fluorescent organic nanocrystals in the aqueous system was stably repeatable. As an extension of this research, this research finding indicates that the fluorescence properties of organic nanocrystals can be controlled using the phase-transitional functional polymer system, where the key factors for stimulation are not only limited to temperature but also light and pH. This fundamental finding of tuneable fluorescence optical property of organic nanocrystals will have several applications such as thermosensitive fluorescence bioimaging of living cells/tissues using PNIPAM-based fluorescent dye nanocrystals; the on–off switching logic gate for optical devices; and medical treatment by photodynamic therapy using PNIPAM-based on-off switching photosensitizing nanocrystals, where the drug efficacy can be controlled by temperature on demand. We believe this finding will be applied in multidisciplinary fields such as nanomedicine, nanobiology, tissue engineering, regenetic medicine, and applied optical physics.
5. Recent topics of organic nanocrystals achieved by several groups
Now a day, with using the reprecipitation method, a series of functional organic nanocrystals/nanoparticles were successfully fabricated by several research groups. For example, nanocrystals from perylene and a perylene derivative were prepared and the spectroscopies of single nanoparticles were studied. Nanoparticles were prepared from
nanocrystals, recently Park’ group reported a phenomenon named aggregation induced enhanced emission (AIEE). Here, enhanced emission instead of fluorescence quenching was observed in the solid state for some specific fluorophores. In general, the fluorescence efficiency of organic chromophores decreases in the solid state, as a result of concentration quenching, even though they show high fluorescence efficiency in solution. Park’s group reported AIEE from organic nanoparticle. First, Park’s group synthesized the organicmolecule 1-cyano-trans-1,2-bis-(40-methylbiphenyl)ethylene (CN-MBE), and then prepared the corresponding nanoparticles. It was interesting that although the fluorescent from CN-MBE solution was quite weak, the nanoparticles emitted a quite strong photoluminescence. It was considered that the aggregation induced the planarization of the CN-MBE molecules in the nanoparticles, which in turn resulted in the strong intermolecular interactions causing a specific aggregation that was good for efficient emission. This phenomenon was specific to nanoparticles and not to bulky crystals.
Not only the above mentioned optical properties, but also some other optoelectronic properties of organic nanomaterials have been reported in recently. For example, the electronic conductance through organic nanowires was investigated. The Tetracyanoquinodimethane (TCNQ) charge transfer complexes nanowires and field emission properties of tris(8-hydroxyquinolino)-aluminum (Alq 3) nanowires were reported. The field-effect transistors (FETs) based on single-crystalline organic one-dimensional nanomaterials were fabricated, and also lasers have proved to be another promising application for organic one-dimensional nanomaterials. The optical waveguiding properties of organic nanowires were reported. The details are well reviewed in the literature written by Yao’s group (Zhao, et al., 2008).
In this chapter, first we explained the preparation method of organic nanocrystals and their improved ones. The reprecipitation method is very useful technique for fabricating several kinds of functional organic nanocrystals. Supercritical fluid crystallization method, microwave-irradiation method, and mass production method extend the potential of the reprecipitation method. Then, several kinds of functional organic nanocrystals including recent topics achieved by several research groups were introduced. The research trend of functional organic nanocrystals had begun with a series of optoelectronic materials, and recently several functional organic nanocrystals were revealed to be useful for nanomedicine such as drug delivery system using pure nanocrystal form of drugs as well as organic solvent free confocal fluorescence imaging of living cells
An B.-K. Kwon S.-K. Jung S.-D. Park S. Y. 2002. Enhanced emission and its switching in fluorescent organic nanoparticles. . 124 48, (November 8, 2002), 14410 14415 0002-7863
Baba K. Kasai H. Okada S. Oikawa H. Nakanishi H. 2000 Novel fabrication process of organic microcrystals using microwave-irradiation., 39 12A(October 16, 2000), L1256 L1258, 0021-4922
Baba K. Kasai H. Okada S. Nakanishi H. Oikawa H. 2006 Fabrication of diacetylene nanofibers and their dynamic behavior in the course of solid-state polymerization. , 445 161 166, 1542-1406
Baba K. Kasai H. Masuhara A. Okada S. Oikawa H. Nakanishi H. 2007a Diacetylene nanowire crystals prepared by reprecipitation/microwave-irradiation method., 46 11(November 6, 2007), 7558 7561, 0021-4922
Baba K. Pudavar H. E. Roy I. Ochulchanskyy T. Y. Chen Y. Pandey R. K. Prasad P. N. 2007b New method for delivering a hydrophobic drug for photodynamic therapy using pure nanocrystal form of the drug. 4 2(February 1, 2007), 289 297, 1543-8384
Baba K. Kasai H. Shinohara Y. Okada S. Oikawa H. Matsuda H. Nakanishi H. 2008 Chemical doping into nanocrystals of poly(diacetylene)., 47 5(May 16, 2008), 3769 3771
Baba K. Kasai H. Masuhara A. Oikawa H. Nakanishi H. 2009 Organic solvent-free fluorescence confocal imaging of living cells using pure nanocrystal forms of fluorescent dyes. 48 11November 20, 2009), 1170021-117002/4
Baba K. Kasai H. Nishida K. Nakanishi H. 2010 Organic Nanocrystals for Nanomedicine and Biophotonics, In: M. Yoshitake, (Ed.), 311 326, Sciyo, 978-9-53307-126-8Vukovar, Croatia
Baba K. Kasai H. Nishida K. Nakanishi H. 2011 Poly(N-isopropylacrylamide)-based thermoresponsive behavior of fluorescent organic nanocrystals. 50(January 5, 2011), 0102021-010202-3
Chen G. Hoffman A. S. 1995 Graft copolymers that exhibit temperature-induced phase transitions over a wide range of pH. 373 6509(05 January 1995), 49 52, 0028-0836
Fu H. Yao J. J. 2001 Size effects on the optical properties of organic nanoparticles. 123 7(January 23, 2001), 1434 1439, 0002-7863
Granqvist C. G. Buhrman R. A. 1976 Ultrafine metal particles. , 47 5(May, 1976), 2200 2219
Heskinsa M. Guillet J. E. 1968 Solution properties of poly(N-isopropylacrylamide). 2 8 1441 1455, 0002-2233X
Ishizaka T. Kasai H. Oikawa H. Nakanishi H. 2006 Unique luminescence properties of Eu3+-doped polyimide., A: Chemistry, 183 3(25 October 2006) 280 284, 1010-6030
Kaneko Yuji. Shimada Satoru. Fukuda Takashi. Kimura Tatsumi. Yokoi Hiroyuki. Matsuda Hiro. Onodera Tsunenobu. Kasai Hitoshi. Okada Shuji. Oikawa Hidetoshi. Nakanishi H. 2005 A novel method for fixing the anisotropic orientation of dispersed organic nanocrystals in a magnetic field. , 17 2 160 163, 0935-9648
Kasai H. Nalwa H. S. Oikawa H. Okada S. Matsuda H. Minami N. Kakuta A. Ono K. Mukho A. Nakanishi H. 1992 A novel preparation method of organic microcrystals. 31 8A(May 29, 1992), L1132 L1134, 0021-4922
Kasai H. Kanbara H. Iida R. Okada S. Matsuda H. Oikawa H. Nakanishi H. 1995 Optical Kerr shutter response of organic microcrystals., 34 9B(August 11, 1995), L1208 L1210, 0021-4922
Kasai H. Kamatani H. Okada S. Oikawa H. Matsuda H. Nakanishi H. 1996 Size-dependent colors and luminescences of organic microcrystals., 35 2B(January 8, 1996), L221 L223, 0021-4922
Katagi H. Kasai H. Okada S. Oikawa H. Komatsu K. Matsuda H. Liu Z. F. Nakanishi H. 1996 Size control of polydiacetylene microcrystals., 3510B, (August 28, 1996), L1364 L1366, 0021-4922
Komai Y. Kasai H. Hirakoso H. Hakuta Y. Okada S. Oikawa H. Adschiri T. Inomata H. Arai K. Nakanishi H. 1998 Size and form control of titanylphthalocyanine microcrystals by supercritical fluid crystallization method., 322(01 November 1998), 167 172, 0105-8725X
Markowicz P. P. Tiryaki H. Pudavar H. Prasad P. N. 2004 Dramatic enhancement of third-harmonic generation in three-dimensional photonic crystals. , 92 8(26 February, 2004), 083903 0031-9007
Matsuda H. Okada S. Masaki A. Nakanishi H. Suda Y. Shigehara K. Yamada A. 1990 Molecular structural view on the large third order nonlinearity of phthalocyanine derivatives, , 1337 105 113, San Diego, CA, USA, (1 December, 1990)
Matsui A. Mizuno K. Nishi O. Matsushima Y. Shimizu M. 1995 Densities of states and bandwidths of excitons in anthracene microcrystallites embedded in PMMA., 194 1(May 1, 1995), 167 174, 0301-0104
Miyashita Y. Baba K. Kasai H. Nakanishi H. Miyashita T. 2008 A new production process of organic pigment nanocrystals., 492 268 274, 1542-1406
Murray C. B. Morris D. J. Bawendi M. G. 1993 Synthesis and characterization of nearly monodisperse CdE (E = sulfur, selenium, tellurium) semiconductor nanocrystallites., 115 19(March 22, 1993), 8706 8715, 0002-7863
Nakamura A. Tokizaki T. Akiyama H. Kataoka T. 1992 Quantum size effects and optical nonlinearity of confined excitons in semiconducting microcrystallites., 53 1-6, (July 1992), 105 109, 0022-2313
Nakanishi H. Katagi H. 1998 Microcrystals of polydiacetylene derivatives and their linear and nonlinear optical properties. , 5 3-4, 289 295
Nishida K. Yamato M. Hayashida Y. Watanabe K. Yamanoto K. Adachi E. Nagai S. Kikuchi A. Maeda N. Watanabe H. Okano T. Tano Y. 2004 Corneal reconstruction with tissue-engineered cell sheets composed of autologous oral mucosal epithelium., 351 12(September 16, 2004), 1187 1196, 0028-4793
Takahashi S. Miura H. Kasai H. Okada S. Nakanishi H. Oikawa H. 2002 Single-crystal-to-single-crystal transformation of diolefin derivatives in nanocrystals. , 124 37(August 24, 2002), 10944 10945), 0002-7863
Tan Z. Masuhara A. Kasai H. Nakanishi H. Oikawa H. 2008 Multibranched C60 micro/nanocrystals fabricated by reprecipitation method. , 47 2Pt. 2, 1426 1428
Tiryaki H. Baba K. Markowicz P. P. Prasad P. N. 2004 Linear and nonlinear optical studies in photonic crystal alloys. , 29 19(October 1, 2004), 2276 2278, 0146-9592
Ujiiye-Ishii K. Baba K. Wei Z. Kasai H. Nakanishi H. Okada S. Oikawa H. 2006 Mass-production of pigment nanocrystals by the reprecipitation method and their encapsulation. , 445 177 183, 1542-1406
Ung T. Giersig M. Dunstan D. Mulvaney P. 1997 Spectroelectrochemistry of colloidal silver., 13 6(March 19, 1997), 1773 1782, 0743-7463
Wei Z. Miura H. Masuhara A. Kasai H. Okada S. Nakanishi H. 2003 Monodispersed poly diacetylene-polystyrene composite particles. 42 10A(October 1, 2003), L1213 L1215
Yanagawa T. Kurokawa Y. Kasai H. Nakanishi H. 1997 Degenerate four-wave mixing using an optical parametric oscillator as an incoherent light source., 137 1-3, (15 April 1997), 103 106, 0030-4018
Zhao G. Ishizaka T. Kasai H. Hasegawa M. Furukawa T. Nakanishi H. Oikawa H. 2009 Ultralow-dielectric-constant films prepared from hollow polyimide nanoparticles possessing controllable core sizes. , 21(29 December, 2008), 419 424, 0897-4756
Zhao Y. S. Fu H. Peng A. Ma Y. Xiao D. Yao J. 2008 Low-dimensional nanomaterials based on small organic molecules: preparation and optoelectronic properties. , 20 15(4 JUL 2008) 2859 2876, 0935-9648